#------------------------------------------------------------------------------
#$Date: 2025-11-29 21:22:08 +0100 (Sat 29 de Nov de 2025) $
#$Revision: 303750 $
#$URL: svn://www.crystallography.net/cod/cif/7/71/96/7719610.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7719610
loop_
_publ_author_name
'Solokha, P.'
'Skachko, D.'
'Freccero, R.'
'Kortus, J.'
'Gumeniuk, R.'
'De Negri, S.'
_publ_section_title
;
 RCuMg₂ compounds (R = Dy-Tm, Lu): crystal
 structure, chemical bonding and magnetic properties.
;
_journal_issue                   43
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16014
_journal_page_last               16027
_journal_paper_doi               10.1039/d5dt01632k
_journal_volume                  54
_journal_year                    2025
_chemical_formula_moiety         'Cu4 Dy4, 8(Mg)'
_chemical_formula_sum            'Cu Dy Mg2'
_chemical_formula_weight         274.66
_space_group_crystal_system      orthorhombic
_space_group_IT_number           51
_space_group_name_Hall           '-P 2a 2a'
_space_group_name_H-M_alt        'P m m a'
_audit_creation_method           SHELXL-2019/1
_audit_update_record
;
2024-09-03 deposited with the CCDC.	2025-09-29 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.5397(4)
_cell_length_b                   3.75940(10)
_cell_length_c                   13.7985(4)
_cell_measurement_reflns_used    1158
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.459
_cell_measurement_theta_min      2.952
_cell_volume                     702.36(3)
_computing_structure_refinement  'SHELXL-2019/1 (Sheldrick, 2019)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'PHOTON III'
_diffrn_measurement_method       'four ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0311
_diffrn_reflns_av_unetI/netI     0.0150
_diffrn_reflns_Laue_measured_fraction_full 0.990
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            14099
_diffrn_reflns_point_group_measured_fraction_full 0.990
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.459
_diffrn_reflns_theta_min         2.952
_exptl_absorpt_coefficient_mu    27.234
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            'metallic grey'
_exptl_crystal_density_diffrn    5.195
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregularly shaped'
_exptl_crystal_F_000             952
_exptl_crystal_size_max          0.045
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.015
_exptl_transmission_factor_max   0.7461
_exptl_transmission_factor_min   0.4342
_refine_diff_density_max         1.023
_refine_diff_density_min         -1.689
_refine_diff_density_rms         0.206
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.180
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     53
_refine_ls_number_reflns         1259
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.180
_refine_ls_R_factor_all          0.0232
_refine_ls_R_factor_gt           0.0201
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0077P)²+6.2174P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0436
_refine_ls_wR_factor_ref         0.0448
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1158
_reflns_number_total             1259
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d5dt01632k2.cif
_cod_data_source_block           PS_1_DyCuMg2_new_0ma_a
_cod_depositor_comments          'Adding full bibliography for 7719610.cif.'
_cod_database_code               7719610
_shelx_shelxl_version_number     2019/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z'
'-x, y, -z'
'x+1/2, -y, -z'
'-x, -y, -z'
'x-1/2, y, -z'
'x, -y, z'
'-x-1/2, y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Dy01 Dy 0.54785(2) 1.000000 0.62396(2) 0.01301(7) Uani 1 2 d S T P . .
Dy02 Dy 0.750000 0.000000 0.81716(3) 0.01510(9) Uani 1 4 d S T P . .
Dy03 Dy 0.750000 0.000000 0.42290(3) 0.01619(9) Uani 1 4 d S T P . .
Cu04 Cu 0.59222(5) 0.500000 0.46644(5) 0.01454(14) Uani 1 2 d S T P . .
Cu05 Cu 0.59149(6) 0.500000 0.78127(5) 0.01633(15) Uani 1 2 d S T P . .
Mg06 Mg 0.49022(16) 0.000000 0.87744(15) 0.0181(4) Uani 1 2 d S T P . .
Mg07 Mg 0.750000 0.500000 0.6212(2) 0.0155(5) Uani 1 4 d S T P . .
Mg08 Mg 0.62450(16) 0.500000 0.26194(15) 0.0186(4) Uani 1 2 d S T P . .
Mg09 Mg 0.63376(17) 0.500000 0.98620(15) 0.0194(4) Uani 1 2 d S T P . .
Mg0A Mg 0.750000 0.000000 0.1301(2) 0.0211(6) Uani 1 4 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Cu05 Dy01 Cu05 79.763(19) . 1_565 ?
Cu05 Dy01 Cu04 95.533(14) . . ?
Cu05 Dy01 Cu04 156.57(2) 1_565 . ?
Cu05 Dy01 Cu04 156.57(2) . 1_565 ?
Cu05 Dy01 Cu04 95.534(14) 1_565 1_565 ?
Cu04 Dy01 Cu04 79.625(18) . 1_565 ?
Cu05 Dy01 Cu04 91.956(15) . 5_666 ?
Cu05 Dy01 Cu04 148.43(2) 1_565 5_666 ?
Cu04 Dy01 Cu04 53.84(2) . 5_666 ?
Cu04 Dy01 Cu04 103.100(13) 1_565 5_666 ?
Cu05 Dy01 Cu04 148.43(2) . 5_676 ?
Cu05 Dy01 Cu04 91.955(15) 1_565 5_676 ?
Cu04 Dy01 Cu04 103.100(13) . 5_676 ?
Cu04 Dy01 Cu04 53.84(2) 1_565 5_676 ?
Cu04 Dy01 Cu04 79.255(19) 5_666 5_676 ?
Cu05 Dy01 Mg07 101.85(4) . 1_565 ?
Cu05 Dy01 Mg07 58.63(5) 1_565 1_565 ?
Cu04 Dy01 Mg07 100.67(4) . 1_565 ?
Cu04 Dy01 Mg07 57.34(5) 1_565 1_565 ?
Cu04 Dy01 Mg07 152.44(5) 5_666 1_565 ?
Cu04 Dy01 Mg07 99.47(2) 5_676 1_565 ?
Cu05 Dy01 Mg07 58.63(5) . . ?
Cu05 Dy01 Mg07 101.86(4) 1_565 . ?
Cu04 Dy01 Mg07 57.34(5) . . ?
Cu04 Dy01 Mg07 100.67(4) 1_565 . ?
Cu04 Dy01 Mg07 99.47(2) 5_666 . ?
Cu04 Dy01 Mg07 152.44(5) 5_676 . ?
Mg07 Dy01 Mg07 68.954(6) 1_565 . ?
Cu05 Dy01 Mg08 55.84(4) . 5_666 ?
Cu05 Dy01 Mg08 98.66(3) 1_565 5_666 ?
Cu04 Dy01 Mg08 97.46(3) . 5_666 ?
Cu04 Dy01 Mg08 147.25(4) 1_565 5_666 ?
Cu04 Dy01 Mg08 53.06(4) 5_666 5_666 ?
Cu04 Dy01 Mg08 96.17(3) 5_676 5_666 ?
Mg07 Dy01 Mg08 152.62(6) 1_565 5_666 ?
Mg07 Dy01 Mg08 105.03(4) . 5_666 ?
Cu05 Dy01 Mg08 98.66(3) . 5_676 ?
Cu05 Dy01 Mg08 55.84(4) 1_565 5_676 ?
Cu04 Dy01 Mg08 147.25(4) . 5_676 ?
Cu04 Dy01 Mg08 97.46(3) 1_565 5_676 ?
Cu04 Dy01 Mg08 96.17(3) 5_666 5_676 ?
Cu04 Dy01 Mg08 53.06(4) 5_676 5_676 ?
Mg07 Dy01 Mg08 105.03(4) 1_565 5_676 ?
Mg07 Dy01 Mg08 152.62(6) . 5_676 ?
Mg08 Dy01 Mg08 67.47(4) 5_666 5_676 ?
Cu05 Dy01 Mg06 47.25(2) . 1_565 ?
Cu05 Dy01 Mg06 47.25(2) 1_565 1_565 ?
Cu04 Dy01 Mg06 140.101(10) . 1_565 ?
Cu04 Dy01 Mg06 140.102(10) 1_565 1_565 ?
Cu04 Dy01 Mg06 105.84(3) 5_666 1_565 ?
Cu04 Dy01 Mg06 105.84(3) 5_676 1_565 ?
Mg07 Dy01 Mg06 101.00(6) 1_565 1_565 ?
Mg07 Dy01 Mg06 101.00(6) . 1_565 ?
Mg08 Dy01 Mg06 52.84(4) 5_666 1_565 ?
Mg08 Dy01 Mg06 52.84(4) 5_676 1_565 ?
Cu05 Dy01 Dy01 139.802(10) . 5_676 ?
Cu05 Dy01 Dy01 139.802(10) 1_565 5_676 ?
Cu04 Dy01 Dy01 51.690(13) . 5_676 ?
Cu04 Dy01 Dy01 51.690(13) 1_565 5_676 ?
Cu04 Dy01 Dy01 51.410(12) 5_666 5_676 ?
Cu04 Dy01 Dy01 51.410(13) 5_676 5_676 ?
Mg07 Dy01 Dy01 106.33(5) 1_565 5_676 ?
Mg07 Dy01 Dy01 106.33(5) . 5_676 ?
Mg08 Dy01 Dy01 101.00(4) 5_666 5_676 ?
Mg08 Dy01 Dy01 101.00(4) 5_676 5_676 ?
Mg06 Dy01 Dy01 146.68(4) 1_565 5_676 ?
Cu05 Dy02 Cu05 80.95(2) . 1_545 ?
Cu05 Dy02 Cu05 95.67(2) . 2_665 ?
Cu05 Dy02 Cu05 160.31(3) 1_545 2_665 ?
Cu05 Dy02 Cu05 160.31(3) . 2_655 ?
Cu05 Dy02 Cu05 95.67(2) 1_545 2_655 ?
Cu05 Dy02 Cu05 80.954(19) 2_665 2_655 ?
Cu05 Dy02 Mg07 103.30(2) . 1_545 ?
Cu05 Dy02 Mg07 59.28(2) 1_545 1_545 ?
Cu05 Dy02 Mg07 103.30(2) 2_665 1_545 ?
Cu05 Dy02 Mg07 59.28(2) 2_655 1_545 ?
Cu05 Dy02 Mg07 59.27(2) . . ?
Cu05 Dy02 Mg07 103.30(2) 1_545 . ?
Cu05 Dy02 Mg07 59.28(2) 2_665 . ?
Cu05 Dy02 Mg07 103.30(2) 2_655 . ?
Mg07 Dy02 Mg07 69.61(6) 1_545 . ?
Cu05 Dy02 Mg09 54.02(4) . . ?
Cu05 Dy02 Mg09 97.68(4) 1_545 . ?
Cu05 Dy02 Mg09 95.86(3) 2_665 . ?
Cu05 Dy02 Mg09 145.40(4) 2_655 . ?
Mg07 Dy02 Mg09 152.01(4) 1_545 . ?
Mg07 Dy02 Mg09 104.42(4) . . ?
Cu05 Dy02 Mg09 95.86(3) . 2_665 ?
Cu05 Dy02 Mg09 145.40(4) 1_545 2_665 ?
Cu05 Dy02 Mg09 54.02(4) 2_665 2_665 ?
Cu05 Dy02 Mg09 97.68(4) 2_655 2_665 ?
Mg07 Dy02 Mg09 152.01(4) 1_545 2_665 ?
Mg07 Dy02 Mg09 104.42(4) . 2_665 ?
Mg09 Dy02 Mg09 55.43(7) . 2_665 ?
Cu05 Dy02 Mg09 145.40(4) . 2_655 ?
Cu05 Dy02 Mg09 95.86(3) 1_545 2_655 ?
Cu05 Dy02 Mg09 97.68(4) 2_665 2_655 ?
Cu05 Dy02 Mg09 54.02(4) 2_655 2_655 ?
Mg07 Dy02 Mg09 104.42(4) 1_545 2_655 ?
Mg07 Dy02 Mg09 152.01(4) . 2_655 ?
Mg09 Dy02 Mg09 92.85(6) . 2_655 ?
Mg09 Dy02 Mg09 67.49(4) 2_665 2_655 ?
Cu05 Dy02 Mg09 97.69(4) . 1_545 ?
Cu05 Dy02 Mg09 54.02(4) 1_545 1_545 ?
Cu05 Dy02 Mg09 145.40(4) 2_665 1_545 ?
Cu05 Dy02 Mg09 95.86(3) 2_655 1_545 ?
Mg07 Dy02 Mg09 104.42(4) 1_545 1_545 ?
Mg07 Dy02 Mg09 152.01(4) . 1_545 ?
Mg09 Dy02 Mg09 67.49(4) . 1_545 ?
Mg09 Dy02 Mg09 92.85(6) 2_665 1_545 ?
Mg09 Dy02 Mg09 55.43(7) 2_655 1_545 ?
Cu05 Dy02 Mg06 47.00(2) . . ?
Cu05 Dy02 Mg06 47.00(2) 1_545 . ?
Cu05 Dy02 Mg06 139.522(10) 2_665 . ?
Cu05 Dy02 Mg06 139.522(10) 2_655 . ?
Mg07 Dy02 Mg06 100.89(3) 1_545 . ?
Mg07 Dy02 Mg06 100.89(3) . . ?
Mg09 Dy02 Mg06 52.32(4) . . ?
Mg09 Dy02 Mg06 107.10(5) 2_665 . ?
Mg09 Dy02 Mg06 107.10(5) 2_655 . ?
Mg09 Dy02 Mg06 52.32(4) 1_545 . ?
Cu05 Dy02 Mg06 139.522(10) . 2_655 ?
Cu05 Dy02 Mg06 139.522(10) 1_545 2_655 ?
Cu05 Dy02 Mg06 47.00(2) 2_665 2_655 ?
Cu05 Dy02 Mg06 47.00(2) 2_655 2_655 ?
Mg07 Dy02 Mg06 100.89(3) 1_545 2_655 ?
Mg07 Dy02 Mg06 100.89(3) . 2_655 ?
Mg09 Dy02 Mg06 107.10(5) . 2_655 ?
Mg09 Dy02 Mg06 52.32(4) 2_665 2_655 ?
Mg09 Dy02 Mg06 52.32(4) 2_655 2_655 ?
Mg09 Dy02 Mg06 107.10(5) 1_545 2_655 ?
Mg06 Dy02 Mg06 153.39(7) . 2_655 ?
Cu04 Dy03 Cu04 156.16(3) 2_665 1_545 ?
Cu04 Dy03 Cu04 80.530(18) 2_665 2_655 ?
Cu04 Dy03 Cu04 94.54(2) 1_545 2_655 ?
Cu04 Dy03 Cu04 94.54(2) 2_665 . ?
Cu04 Dy03 Cu04 80.530(18) 1_545 . ?
Cu04 Dy03 Cu04 156.16(3) 2_655 . ?
Cu04 Dy03 Mg07 57.57(2) 2_665 . ?
Cu04 Dy03 Mg07 101.29(2) 1_545 . ?
Cu04 Dy03 Mg07 101.29(2) 2_655 . ?
Cu04 Dy03 Mg07 57.57(2) . . ?
Cu04 Dy03 Mg07 101.29(2) 2_665 1_545 ?
Cu04 Dy03 Mg07 57.57(2) 1_545 1_545 ?
Cu04 Dy03 Mg07 57.57(2) 2_655 1_545 ?
Cu04 Dy03 Mg07 101.29(2) . 1_545 ?
Mg07 Dy03 Mg07 68.98(6) . 1_545 ?
Cu04 Dy03 Mg08 150.13(4) 2_665 1_545 ?
Cu04 Dy03 Mg08 53.50(4) 1_545 1_545 ?
Cu04 Dy03 Mg08 98.40(3) 2_655 1_545 ?
Cu04 Dy03 Mg08 97.25(3) . 1_545 ?
Mg07 Dy03 Mg08 149.22(4) . 1_545 ?
Mg07 Dy03 Mg08 103.14(3) 1_545 1_545 ?
Cu04 Dy03 Mg08 97.25(3) 2_665 2_655 ?
Cu04 Dy03 Mg08 98.40(3) 1_545 2_655 ?
Cu04 Dy03 Mg08 53.50(4) 2_655 2_655 ?
Cu04 Dy03 Mg08 150.13(4) . 2_655 ?
Mg07 Dy03 Mg08 149.22(4) . 2_655 ?
Mg07 Dy03 Mg08 103.14(3) 1_545 2_655 ?
Mg08 Dy03 Mg08 60.57(7) 1_545 2_655 ?
Cu04 Dy03 Mg08 53.50(4) 2_665 2_665 ?
Cu04 Dy03 Mg08 150.13(4) 1_545 2_665 ?
Cu04 Dy03 Mg08 97.25(3) 2_655 2_665 ?
Cu04 Dy03 Mg08 98.40(3) . 2_665 ?
Mg07 Dy03 Mg08 103.14(3) . 2_665 ?
Mg07 Dy03 Mg08 149.22(4) 1_545 2_665 ?
Mg08 Dy03 Mg08 97.53(6) 1_545 2_665 ?
Mg08 Dy03 Mg08 67.81(4) 2_655 2_665 ?
Cu04 Dy03 Mg08 98.40(3) 2_665 . ?
Cu04 Dy03 Mg08 97.25(3) 1_545 . ?
Cu04 Dy03 Mg08 150.13(4) 2_655 . ?
Cu04 Dy03 Mg08 53.50(4) . . ?
Mg07 Dy03 Mg08 103.14(3) . . ?
Mg07 Dy03 Mg08 149.22(4) 1_545 . ?
Mg08 Dy03 Mg08 67.81(4) 1_545 . ?
Mg08 Dy03 Mg08 97.53(6) 2_655 . ?
Mg08 Dy03 Mg08 60.57(7) 2_665 . ?
Cu04 Dy03 Dy03 49.735(9) 2_665 1_565 ?
Cu04 Dy03 Dy03 130.265(9) 1_545 1_565 ?
Cu04 Dy03 Dy03 130.265(9) 2_655 1_565 ?
Cu04 Dy03 Dy03 49.735(9) . 1_565 ?
Mg07 Dy03 Dy03 55.51(3) . 1_565 ?
Mg07 Dy03 Dy03 124.49(3) 1_545 1_565 ?
Mg08 Dy03 Dy03 123.91(2) 1_545 1_565 ?
Mg08 Dy03 Dy03 123.91(2) 2_655 1_565 ?
Mg08 Dy03 Dy03 56.09(2) 2_665 1_565 ?
Mg08 Dy03 Dy03 56.09(2) . 1_565 ?
Cu04 Dy03 Dy03 130.265(9) 2_665 1_545 ?
Cu04 Dy03 Dy03 49.735(9) 1_545 1_545 ?
Cu04 Dy03 Dy03 49.735(9) 2_655 1_545 ?
Cu04 Dy03 Dy03 130.265(9) . 1_545 ?
Mg07 Dy03 Dy03 124.49(3) . 1_545 ?
Mg07 Dy03 Dy03 55.51(3) 1_545 1_545 ?
Mg08 Dy03 Dy03 56.09(2) 1_545 1_545 ?
Mg08 Dy03 Dy03 56.09(2) 2_655 1_545 ?
Mg08 Dy03 Dy03 123.91(2) 2_665 1_545 ?
Mg08 Dy03 Dy03 123.91(2) . 1_545 ?
Dy03 Dy03 Dy03 180.0 1_565 1_545 ?
Cu04 Cu04 Mg08 119.15(6) 5_666 . ?
Cu04 Cu04 Dy03 139.513(10) 5_666 . ?
Mg08 Cu04 Dy03 71.54(4) . . ?
Cu04 Cu04 Dy03 139.514(10) 5_666 1_565 ?
Mg08 Cu04 Dy03 71.54(4) . 1_565 ?
Dy03 Cu04 Dy03 80.530(18) . 1_565 ?
Cu04 Cu04 Dy01 63.30(2) 5_666 1_545 ?
Mg08 Cu04 Dy01 139.728(12) . 1_545 ?
Dy03 Cu04 Dy01 83.651(12) . 1_545 ?
Dy03 Cu04 Dy01 135.81(3) 1_565 1_545 ?
Cu04 Cu04 Dy01 63.30(2) 5_666 . ?
Mg08 Cu04 Dy01 139.728(12) . . ?
Dy03 Cu04 Dy01 135.81(3) . . ?
Dy03 Cu04 Dy01 83.652(12) 1_565 . ?
Dy01 Cu04 Dy01 79.625(18) 1_545 . ?
Cu04 Cu04 Dy01 62.86(2) 5_666 5_666 ?
Mg08 Cu04 Dy01 71.35(4) . 5_666 ?
Dy03 Cu04 Dy01 88.455(10) . 5_666 ?
Dy03 Cu04 Dy01 142.89(3) 1_565 5_666 ?
Dy01 Cu04 Dy01 76.899(13) 1_545 5_666 ?
Dy01 Cu04 Dy01 126.16(2) . 5_666 ?
Cu04 Cu04 Dy01 62.86(2) 5_666 5_676 ?
Mg08 Cu04 Dy01 71.35(4) . 5_676 ?
Dy03 Cu04 Dy01 142.89(3) . 5_676 ?
Dy03 Cu04 Dy01 88.454(10) 1_565 5_676 ?
Dy01 Cu04 Dy01 126.16(2) 1_545 5_676 ?
Dy01 Cu04 Dy01 76.899(13) . 5_676 ?
Dy01 Cu04 Dy01 79.255(19) 5_666 5_676 ?
Cu04 Cu04 Mg07 114.67(5) 5_666 . ?
Mg08 Cu04 Mg07 126.18(6) . . ?
Dy03 Cu04 Mg07 68.07(3) . . ?
Dy03 Cu04 Mg07 68.07(3) 1_565 . ?
Dy01 Cu04 Mg07 67.75(3) 1_545 . ?
Dy01 Cu04 Mg07 67.75(3) . . ?
Dy01 Cu04 Mg07 138.968(15) 5_666 . ?
Dy01 Cu04 Mg07 138.968(15) 5_676 . ?
Mg06 Cu05 Mg06 89.14(7) . 1_565 ?
Mg06 Cu05 Mg09 67.42(5) . . ?
Mg06 Cu05 Mg09 67.42(5) 1_565 . ?
Mg06 Cu05 Dy02 80.74(4) . . ?
Mg06 Cu05 Dy02 138.61(5) 1_565 . ?
Mg09 Cu05 Dy02 71.66(4) . . ?
Mg06 Cu05 Dy02 138.61(5) . 1_565 ?
Mg06 Cu05 Dy02 80.74(4) 1_565 1_565 ?
Mg09 Cu05 Dy02 71.66(4) . 1_565 ?
Dy02 Cu05 Dy02 80.954(19) . 1_565 ?
Mg06 Cu05 Dy01 135.53(5) . . ?
Mg06 Cu05 Dy01 79.26(4) 1_565 . ?
Mg09 Cu05 Dy01 139.969(11) . . ?
Dy02 Cu05 Dy01 133.81(3) . . ?
Dy02 Cu05 Dy01 81.939(13) 1_565 . ?
Mg06 Cu05 Dy01 79.26(4) . 1_545 ?
Mg06 Cu05 Dy01 135.53(5) 1_565 1_545 ?
Mg09 Cu05 Dy01 139.970(11) . 1_545 ?
Dy02 Cu05 Dy01 81.939(12) . 1_545 ?
Dy02 Cu05 Dy01 133.81(3) 1_565 1_545 ?
Dy01 Cu05 Dy01 79.763(19) . 1_545 ?
Mg06 Cu05 Mg08 66.26(5) . 5_666 ?
Mg06 Cu05 Mg08 66.26(5) 1_565 5_666 ?
Mg09 Cu05 Mg08 112.97(6) . 5_666 ?
Dy02 Cu05 Mg08 139.501(10) . 5_666 ?
Dy02 Cu05 Mg08 139.501(10) 1_565 5_666 ?
Dy01 Cu05 Mg08 69.79(3) . 5_666 ?
Dy01 Cu05 Mg08 69.79(3) 1_545 5_666 ?
Mg06 Cu05 Mg07 135.40(3) . . ?
Mg06 Cu05 Mg07 135.40(3) 1_565 . ?
Mg09 Cu05 Mg07 124.39(6) . . ?
Dy02 Cu05 Mg07 66.81(3) . . ?
Dy02 Cu05 Mg07 66.81(3) 1_565 . ?
Dy01 Cu05 Mg07 67.01(3) . . ?
Dy01 Cu05 Mg07 67.01(3) 1_545 . ?
Mg08 Cu05 Mg07 122.65(6) 5_666 . ?
Cu05 Mg06 Cu05 89.14(7) 1_545 . ?
Cu05 Mg06 Mg09 110.20(8) 1_545 . ?
Cu05 Mg06 Mg09 59.48(5) . . ?
Cu05 Mg06 Mg09 59.48(5) 1_545 1_545 ?
Cu05 Mg06 Mg09 110.20(8) . 1_545 ?
Mg09 Mg06 Mg09 74.87(7) . 1_545 ?
Cu05 Mg06 Mg08 61.60(5) 1_545 5_656 ?
Cu05 Mg06 Mg08 111.96(8) . 5_656 ?
Mg09 Mg06 Mg08 169.35(10) . 5_656 ?
Mg09 Mg06 Mg08 104.30(4) 1_545 5_656 ?
Cu05 Mg06 Mg08 111.96(8) 1_545 5_666 ?
Cu05 Mg06 Mg08 61.60(5) . 5_666 ?
Mg09 Mg06 Mg08 104.30(4) . 5_666 ?
Mg09 Mg06 Mg08 169.35(10) 1_545 5_666 ?
Mg08 Mg06 Mg08 74.50(7) 5_656 5_666 ?
Cu05 Mg06 Mg09 171.52(7) 1_545 5_667 ?
Cu05 Mg06 Mg09 98.64(3) . 5_667 ?
Mg09 Mg06 Mg09 71.45(8) . 5_667 ?
Mg09 Mg06 Mg09 114.10(7) 1_545 5_667 ?
Mg08 Mg06 Mg09 117.73(9) 5_656 5_667 ?
Mg08 Mg06 Mg09 75.04(6) 5_666 5_667 ?
Cu05 Mg06 Mg09 98.64(3) 1_545 5_657 ?
Cu05 Mg06 Mg09 171.52(7) . 5_657 ?
Mg09 Mg06 Mg09 114.11(7) . 5_657 ?
Mg09 Mg06 Mg09 71.45(8) 1_545 5_657 ?
Mg08 Mg06 Mg09 75.04(6) 5_656 5_657 ?
Mg08 Mg06 Mg09 117.73(9) 5_666 5_657 ?
Mg09 Mg06 Mg09 73.41(7) 5_667 5_657 ?
Cu05 Mg06 Mg0A 119.72(7) 1_545 5_656 ?
Cu05 Mg06 Mg0A 119.72(7) . 5_656 ?
Mg09 Mg06 Mg0A 130.06(7) . 5_656 ?
Mg09 Mg06 Mg0A 130.06(7) 1_545 5_656 ?
Mg08 Mg06 Mg0A 58.69(7) 5_656 5_656 ?
Mg08 Mg06 Mg0A 58.69(7) 5_666 5_656 ?
Mg09 Mg06 Mg0A 59.04(7) 5_667 5_656 ?
Mg09 Mg06 Mg0A 59.04(7) 5_657 5_656 ?
Cu05 Mg06 Mg06 117.00(7) 1_545 5_657 ?
Cu05 Mg06 Mg06 117.00(7) . 5_657 ?
Mg09 Mg06 Mg06 57.80(6) . 5_657 ?
Mg09 Mg06 Mg06 57.80(6) 1_545 5_657 ?
Mg08 Mg06 Mg06 131.03(7) 5_656 5_657 ?
Mg08 Mg06 Mg06 131.03(7) 5_666 5_657 ?
Mg09 Mg06 Mg06 56.31(6) 5_667 5_657 ?
Mg09 Mg06 Mg06 56.31(6) 5_657 5_657 ?
Mg0A Mg06 Mg06 96.31(10) 5_656 5_657 ?
Cu05 Mg06 Dy01 53.49(4) 1_545 1_545 ?
Cu05 Mg06 Dy01 53.49(4) . 1_545 ?
Mg09 Mg06 Dy01 109.68(6) . 1_545 ?
Mg09 Mg06 Dy01 109.68(6) 1_545 1_545 ?
Mg08 Mg06 Dy01 60.30(5) 5_656 1_545 ?
Mg08 Mg06 Dy01 60.30(5) 5_666 1_545 ?
Mg09 Mg06 Dy01 134.44(5) 5_667 1_545 ?
Mg09 Mg06 Dy01 134.44(5) 5_657 1_545 ?
Mg0A Mg06 Dy01 100.75(8) 5_656 1_545 ?
Mg06 Mg06 Dy01 162.95(11) 5_657 1_545 ?
Cu05 Mg06 Dy02 52.25(4) 1_545 . ?
Cu05 Mg06 Dy02 52.25(4) . . ?
Mg09 Mg06 Dy02 60.01(5) . . ?
Mg09 Mg06 Dy02 60.01(5) 1_545 . ?
Mg08 Mg06 Dy02 110.13(7) 5_656 . ?
Mg08 Mg06 Dy02 110.13(7) 5_666 . ?
Mg09 Mg06 Dy02 131.08(6) 5_667 . ?
Mg09 Mg06 Dy02 131.08(6) 5_657 . ?
Mg0A Mg06 Dy02 164.86(9) 5_656 . ?
Mg06 Mg06 Dy02 98.83(9) 5_657 . ?
Dy01 Mg06 Dy02 64.12(4) 1_545 . ?
Cu04 Mg07 Cu04 90.03(8) . 2_665 ?
Cu04 Mg07 Cu05 90.810(18) . . ?
Cu04 Mg07 Cu05 179.16(8) 2_665 . ?
Cu04 Mg07 Cu05 179.16(8) . 2_665 ?
Cu04 Mg07 Cu05 90.811(19) 2_665 2_665 ?
Cu05 Mg07 Cu05 88.35(8) . 2_665 ?
Cu04 Mg07 Dy02 125.483(17) . . ?
Cu04 Mg07 Dy02 125.483(17) 2_665 . ?
Cu05 Mg07 Dy02 53.92(4) . . ?
Cu05 Mg07 Dy02 53.92(4) 2_665 . ?
Cu04 Mg07 Dy02 125.483(17) . 1_565 ?
Cu04 Mg07 Dy02 125.483(17) 2_665 1_565 ?
Cu05 Mg07 Dy02 53.92(4) . 1_565 ?
Cu05 Mg07 Dy02 53.92(4) 2_665 1_565 ?
Dy02 Mg07 Dy02 69.60(6) . 1_565 ?
Cu04 Mg07 Dy03 54.36(4) . . ?
Cu04 Mg07 Dy03 54.36(4) 2_665 . ?
Cu05 Mg07 Dy03 126.239(16) . . ?
Cu05 Mg07 Dy03 126.239(16) 2_665 . ?
Dy02 Mg07 Dy03 110.706(6) . . ?
Dy02 Mg07 Dy03 179.69(6) 1_565 . ?
Cu04 Mg07 Dy03 54.36(4) . 1_565 ?
Cu04 Mg07 Dy03 54.36(4) 2_665 1_565 ?
Cu05 Mg07 Dy03 126.239(16) . 1_565 ?
Cu05 Mg07 Dy03 126.239(16) 2_665 1_565 ?
Dy02 Mg07 Dy03 179.69(6) . 1_565 ?
Dy02 Mg07 Dy03 110.707(6) 1_565 1_565 ?
Dy03 Mg07 Dy03 68.98(6) . 1_565 ?
Cu04 Mg07 Dy01 126.24(7) . 2_675 ?
Cu04 Mg07 Dy01 54.913(19) 2_665 2_675 ?
Cu05 Mg07 Dy01 124.48(7) . 2_675 ?
Cu05 Mg07 Dy01 54.36(2) 2_665 2_675 ?
Dy02 Mg07 Dy01 108.28(6) . 2_675 ?
Dy02 Mg07 Dy01 70.57(3) 1_565 2_675 ?
Dy03 Mg07 Dy01 109.28(6) . 2_675 ?
Dy03 Mg07 Dy01 71.88(3) 1_565 2_675 ?
Cu04 Mg07 Dy01 54.913(19) . 1_545 ?
Cu04 Mg07 Dy01 126.24(7) 2_665 1_545 ?
Cu05 Mg07 Dy01 54.36(2) . 1_545 ?
Cu05 Mg07 Dy01 124.48(7) 2_665 1_545 ?
Dy02 Mg07 Dy01 70.57(3) . 1_545 ?
Dy02 Mg07 Dy01 108.28(6) 1_565 1_545 ?
Dy03 Mg07 Dy01 71.88(3) . 1_545 ?
Dy03 Mg07 Dy01 109.27(6) 1_565 1_545 ?
Dy01 Mg07 Dy01 178.67(10) 2_675 1_545 ?
Cu04 Mg07 Dy01 126.24(7) . 2_665 ?
Cu04 Mg07 Dy01 54.913(19) 2_665 2_665 ?
Cu05 Mg07 Dy01 124.48(7) . 2_665 ?
Cu05 Mg07 Dy01 54.36(2) 2_665 2_665 ?
Dy02 Mg07 Dy01 70.57(3) . 2_665 ?
Dy02 Mg07 Dy01 108.27(6) 1_565 2_665 ?
Dy03 Mg07 Dy01 71.88(3) . 2_665 ?
Dy03 Mg07 Dy01 109.27(6) 1_565 2_665 ?
Dy01 Mg07 Dy01 68.955(6) 2_675 2_665 ?
Dy01 Mg07 Dy01 111.029(6) 1_545 2_665 ?
Cu04 Mg07 Dy01 54.913(19) . . ?
Cu04 Mg07 Dy01 126.24(7) 2_665 . ?
Cu05 Mg07 Dy01 54.36(2) . . ?
Cu05 Mg07 Dy01 124.48(7) 2_665 . ?
Dy02 Mg07 Dy01 108.27(6) . . ?
Dy02 Mg07 Dy01 70.57(3) 1_565 . ?
Dy03 Mg07 Dy01 109.28(6) . . ?
Dy03 Mg07 Dy01 71.88(3) 1_565 . ?
Dy01 Mg07 Dy01 111.029(6) 2_675 . ?
Dy01 Mg07 Dy01 68.954(6) 1_545 . ?
Dy01 Mg07 Dy01 178.67(10) 2_665 . ?
Cu04 Mg08 Cu05 92.72(6) . 5_666 ?
Cu04 Mg08 Mg06 122.37(7) . 5_656 ?
Cu05 Mg08 Mg06 52.14(5) 5_666 5_656 ?
Cu04 Mg08 Mg06 122.37(7) . 5_666 ?
Cu05 Mg08 Mg06 52.14(5) 5_666 5_666 ?
Mg06 Mg08 Mg06 74.50(7) 5_656 5_666 ?
Cu04 Mg08 Mg0A 131.28(7) . 1_565 ?
Cu05 Mg08 Mg0A 114.66(6) 5_666 1_565 ?
Mg06 Mg08 Mg0A 106.02(9) 5_656 1_565 ?
Mg06 Mg08 Mg0A 63.03(5) 5_666 1_565 ?
Cu04 Mg08 Mg0A 131.28(7) . . ?
Cu05 Mg08 Mg0A 114.66(6) 5_666 . ?
Mg06 Mg08 Mg0A 63.03(5) 5_656 . ?
Mg06 Mg08 Mg0A 106.02(9) 5_666 . ?
Mg0A Mg08 Mg0A 74.11(7) 1_565 . ?
Cu04 Mg08 Dy03 54.96(4) . 1_565 ?
Cu05 Mg08 Dy03 128.74(5) 5_666 1_565 ?
Mg06 Mg08 Dy03 176.44(5) 5_656 1_565 ?
Mg06 Mg08 Dy03 108.83(2) 5_666 1_565 ?
Mg0A Mg08 Dy03 76.91(6) 1_565 1_565 ?
Mg0A Mg08 Dy03 116.48(7) . 1_565 ?
Cu04 Mg08 Dy03 54.96(4) . . ?
Cu05 Mg08 Dy03 128.74(5) 5_666 . ?
Mg06 Mg08 Dy03 108.83(2) 5_656 . ?
Mg06 Mg08 Dy03 176.44(5) 5_666 . ?
Mg0A Mg08 Dy03 116.48(7) 1_565 . ?
Mg0A Mg08 Dy03 76.91(6) . . ?
Dy03 Mg08 Dy03 67.81(4) 1_565 . ?
Cu04 Mg08 Dy01 55.59(4) . 5_666 ?
Cu05 Mg08 Dy01 54.37(4) 5_666 5_666 ?
Mg06 Mg08 Dy01 66.87(5) 5_656 5_666 ?
Mg06 Mg08 Dy01 106.22(7) 5_666 5_666 ?
Mg0A Mg08 Dy01 168.95(8) 1_565 5_666 ?
Mg0A Mg08 Dy01 108.19(2) . 5_666 ?
Dy03 Mg08 Dy01 110.54(6) 1_565 5_666 ?
Dy03 Mg08 Dy01 74.41(3) . 5_666 ?
Cu04 Mg08 Dy01 55.59(4) . 5_676 ?
Cu05 Mg08 Dy01 54.37(4) 5_666 5_676 ?
Mg06 Mg08 Dy01 106.22(7) 5_656 5_676 ?
Mg06 Mg08 Dy01 66.87(5) 5_666 5_676 ?
Mg0A Mg08 Dy01 108.19(2) 1_565 5_676 ?
Mg0A Mg08 Dy01 168.95(8) . 5_676 ?
Dy03 Mg08 Dy01 74.41(3) 1_565 5_676 ?
Dy03 Mg08 Dy01 110.54(6) . 5_676 ?
Dy01 Mg08 Dy01 67.47(4) 5_666 5_676 ?
Cu04 Mg08 Mg08 98.80(5) . 2_665 ?
Cu05 Mg08 Mg08 168.48(4) 5_666 2_665 ?
Mg06 Mg08 Mg08 120.01(5) 5_656 2_665 ?
Mg06 Mg08 Mg08 120.01(5) 5_666 2_665 ?
Mg0A Mg08 Mg08 56.99(4) 1_565 2_665 ?
Mg0A Mg08 Mg08 56.99(4) . 2_665 ?
Dy03 Mg08 Mg08 59.71(4) 1_565 2_665 ?
Dy03 Mg08 Mg08 59.71(4) . 2_665 ?
Dy01 Mg08 Mg08 133.58(3) 5_666 2_665 ?
Dy01 Mg08 Mg08 133.58(3) 5_676 2_665 ?
Cu05 Mg09 Mg06 53.11(5) . . ?
Cu05 Mg09 Mg06 53.11(5) . 1_565 ?
Mg06 Mg09 Mg06 74.87(7) . 1_565 ?
Cu05 Mg09 Mg06 118.72(7) . 5_667 ?
Mg06 Mg09 Mg06 108.55(8) . 5_667 ?
Mg06 Mg09 Mg06 65.90(7) 1_565 5_667 ?
Cu05 Mg09 Mg06 118.72(7) . 5_657 ?
Mg06 Mg09 Mg06 65.90(7) . 5_657 ?
Mg06 Mg09 Mg06 108.55(8) 1_565 5_657 ?
Mg06 Mg09 Mg06 73.41(7) 5_667 5_657 ?
Cu05 Mg09 Mg09 101.44(5) . 2_665 ?
Mg06 Mg09 Mg09 128.94(5) . 2_665 ?
Mg06 Mg09 Mg09 128.94(5) 1_565 2_665 ?
Mg06 Mg09 Mg09 122.26(5) 5_667 2_665 ?
Mg06 Mg09 Mg09 122.26(5) 5_657 2_665 ?
Cu05 Mg09 Mg0A 135.71(7) . 1_566 ?
Mg06 Mg09 Mg0A 168.86(10) . 1_566 ?
Mg06 Mg09 Mg0A 104.88(3) 1_565 1_566 ?
Mg06 Mg09 Mg0A 62.20(5) 5_667 1_566 ?
Mg06 Mg09 Mg0A 104.23(8) 5_657 1_566 ?
Mg09 Mg09 Mg0A 60.07(4) 2_665 1_566 ?
Cu05 Mg09 Mg0A 135.71(7) . 1_556 ?
Mg06 Mg09 Mg0A 104.88(3) . 1_556 ?
Mg06 Mg09 Mg0A 168.86(10) 1_565 1_556 ?
Mg06 Mg09 Mg0A 104.23(8) 5_667 1_556 ?
Mg06 Mg09 Mg0A 62.20(5) 5_657 1_556 ?
Mg09 Mg09 Mg0A 60.07(4) 2_665 1_556 ?
Mg0A Mg09 Mg0A 73.14(7) 1_566 1_556 ?
Cu05 Mg09 Dy02 54.32(4) . 1_565 ?
Mg06 Mg09 Dy02 107.18(7) . 1_565 ?
Mg06 Mg09 Dy02 67.67(5) 1_565 1_565 ?
Mg06 Mg09 Dy02 109.18(2) 5_667 1_565 ?
Mg06 Mg09 Dy02 173.03(8) 5_657 1_565 ?
Mg09 Mg09 Dy02 62.28(4) 2_665 1_565 ?
Mg0A Mg09 Dy02 82.58(6) 1_566 1_565 ?
Mg0A Mg09 Dy02 122.19(7) 1_556 1_565 ?
Cu05 Mg09 Dy02 54.31(4) . . ?
Mg06 Mg09 Dy02 67.67(5) . . ?
Mg06 Mg09 Dy02 107.18(7) 1_565 . ?
Mg06 Mg09 Dy02 173.03(8) 5_667 . ?
Mg06 Mg09 Dy02 109.19(2) 5_657 . ?
Mg09 Mg09 Dy02 62.28(4) 2_665 . ?
Mg0A Mg09 Dy02 122.19(7) 1_566 . ?
Mg0A Mg09 Dy02 82.58(6) 1_556 . ?
Dy02 Mg09 Dy02 67.49(4) 1_565 . ?
Cu05 Mg09 Mg09 84.56(8) . 5_667 ?
Mg06 Mg09 Mg09 54.95(6) . 5_667 ?
Mg06 Mg09 Mg09 54.95(6) 1_565 5_667 ?
Mg06 Mg09 Mg09 53.61(6) 5_667 5_667 ?
Mg06 Mg09 Mg09 53.61(6) 5_657 5_667 ?
Mg09 Mg09 Mg09 174.00(7) 2_665 5_667 ?
Mg0A Mg09 Mg09 115.49(8) 1_566 5_667 ?
Mg0A Mg09 Mg09 115.49(8) 1_556 5_667 ?
Dy02 Mg09 Mg09 122.32(7) 1_565 5_667 ?
Dy02 Mg09 Mg09 122.32(7) . 5_667 ?
Mg08 Mg0A Mg08 108.64(12) 2_665 1_545 ?
Mg08 Mg0A Mg08 74.11(7) 2_665 2_655 ?
Mg08 Mg0A Mg08 66.01(9) 1_545 2_655 ?
Mg08 Mg0A Mg08 66.01(9) 2_665 . ?
Mg08 Mg0A Mg08 74.11(7) 1_545 . ?
Mg08 Mg0A Mg08 108.64(12) 2_655 . ?
Mg08 Mg0A Mg09 176.26(10) 2_665 1_544 ?
Mg08 Mg0A Mg09 74.71(5) 1_545 1_544 ?
Mg08 Mg0A Mg09 106.25(3) 2_655 1_544 ?
Mg08 Mg0A Mg09 117.02(5) . 1_544 ?
Mg08 Mg0A Mg09 117.02(5) 2_665 2_654 ?
Mg08 Mg0A Mg09 106.25(3) 1_545 2_654 ?
Mg08 Mg0A Mg09 74.71(5) 2_655 2_654 ?
Mg08 Mg0A Mg09 176.25(10) . 2_654 ?
Mg09 Mg0A Mg09 59.86(9) 1_544 2_654 ?
Mg08 Mg0A Mg09 106.25(3) 2_665 1_554 ?
Mg08 Mg0A Mg09 117.02(5) 1_545 1_554 ?
Mg08 Mg0A Mg09 176.26(10) 2_655 1_554 ?
Mg08 Mg0A Mg09 74.71(5) . 1_554 ?
Mg09 Mg0A Mg09 73.15(7) 1_544 1_554 ?
Mg09 Mg0A Mg09 102.00(12) 2_654 1_554 ?
Mg08 Mg0A Mg09 74.71(5) 2_665 2_664 ?
Mg08 Mg0A Mg09 176.26(10) 1_545 2_664 ?
Mg08 Mg0A Mg09 117.02(5) 2_655 2_664 ?
Mg08 Mg0A Mg09 106.25(3) . 2_664 ?
Mg09 Mg0A Mg09 102.00(12) 1_544 2_664 ?
Mg09 Mg0A Mg09 73.15(7) 2_654 2_664 ?
Mg09 Mg0A Mg09 59.86(9) 1_554 2_664 ?
Mg08 Mg0A Mg06 124.27(8) 2_665 5_656 ?
Mg08 Mg0A Mg06 58.28(5) 1_545 5_656 ?
Mg08 Mg0A Mg06 124.27(8) 2_655 5_656 ?
Mg08 Mg0A Mg06 58.27(5) . 5_656 ?
Mg09 Mg0A Mg06 58.75(5) 1_544 5_656 ?
Mg09 Mg0A Mg06 118.59(8) 2_654 5_656 ?
Mg09 Mg0A Mg06 58.75(5) 1_554 5_656 ?
Mg09 Mg0A Mg06 118.59(8) 2_664 5_656 ?
Mg08 Mg0A Mg06 58.28(5) 2_665 6_656 ?
Mg08 Mg0A Mg06 124.27(8) 1_545 6_656 ?
Mg08 Mg0A Mg06 58.28(5) 2_655 6_656 ?
Mg08 Mg0A Mg06 124.27(8) . 6_656 ?
Mg09 Mg0A Mg06 118.59(8) 1_544 6_656 ?
Mg09 Mg0A Mg06 58.75(5) 2_654 6_656 ?
Mg09 Mg0A Mg06 118.59(8) 1_554 6_656 ?
Mg09 Mg0A Mg06 58.75(5) 2_664 6_656 ?
Mg06 Mg0A Mg06 176.34(14) 5_656 6_656 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Dy01 Cu05 2.9315(6) . ?
Dy01 Cu05 2.9315(6) 1_565 ?
Dy01 Cu04 2.9358(6) . ?
Dy01 Cu04 2.9358(6) 1_565 ?
Dy01 Cu04 2.9472(6) 5_666 ?
Dy01 Cu04 2.9472(6) 5_676 ?
Dy01 Mg07 3.3206(2) 1_565 ?
Dy01 Mg07 3.3206(2) . ?
Dy01 Mg08 3.3848(18) 5_666 ?
Dy01 Mg08 3.3848(18) 5_676 ?
Dy01 Mg06 3.584(2) 1_565 ?
Dy01 Dy01 3.6582(5) 5_676 ?
Dy02 Cu05 2.8957(6) . ?
Dy02 Cu05 2.8957(6) 1_545 ?
Dy02 Cu05 2.8957(6) 2_665 ?
Dy02 Cu05 2.8957(6) 2_655 ?
Dy02 Mg07 3.293(2) 1_545 ?
Dy02 Mg07 3.293(2) . ?
Dy02 Mg09 3.3840(18) . ?
Dy02 Mg09 3.3840(18) 2_665 ?
Dy02 Mg09 3.3840(18) 2_655 ?
Dy02 Mg09 3.3840(18) 1_545 ?
Dy02 Mg06 3.614(2) . ?
Dy02 Mg06 3.614(2) 2_655 ?
Dy03 Cu04 2.9083(5) 2_665 ?
Dy03 Cu04 2.9083(5) 1_545 ?
Dy03 Cu04 2.9083(5) 2_655 ?
Dy03 Cu04 2.9083(5) . ?
Dy03 Mg07 3.319(2) . ?
Dy03 Mg07 3.319(2) 1_545 ?
Dy03 Mg08 3.3695(18) 1_545 ?
Dy03 Mg08 3.3695(18) 2_655 ?
Dy03 Mg08 3.3695(18) 2_665 ?
Dy03 Mg08 3.3695(18) . ?
Dy03 Dy03 3.75940(10) 1_565 ?
Dy03 Dy03 3.75940(10) 1_545 ?
Cu04 Cu04 2.6634(14) 5_666 ?
Cu04 Mg08 2.855(2) . ?
Cu04 Mg07 3.020(2) . ?
Cu05 Mg06 2.6785(16) . ?
Cu05 Mg06 2.6785(16) 1_565 ?
Cu05 Mg09 2.885(2) . ?
Cu05 Mg08 2.985(2) 5_666 ?
Cu05 Mg07 3.080(2) . ?
Mg06 Mg09 3.092(2) . ?
Mg06 Mg09 3.092(2) 1_545 ?
Mg06 Mg08 3.106(2) 5_656 ?
Mg06 Mg08 3.106(2) 5_666 ?
Mg06 Mg09 3.145(2) 5_667 ?
Mg06 Mg09 3.145(2) 5_657 ?
Mg06 Mg0A 3.254(2) 5_656 ?
Mg06 Mg06 3.393(4) 5_657 ?
Mg08 Mg0A 3.119(3) 1_565 ?
Mg08 Mg0A 3.119(3) . ?
Mg08 Mg08 3.399(4) 2_665 ?
Mg09 Mg09 3.148(5) 2_665 ?
Mg09 Mg0A 3.155(3) 1_566 ?
Mg09 Mg0A 3.155(3) 1_556 ?
Mg09 Mg09 3.642(5) 5_667 ?
